Home | About | Journals | Submit | Contact Us | Français |

**|**Nanoscale Res Lett**|**v.4(12); 2009**|**PMC2893785

Formats

Article sections

Authors

Related links

Nanoscale Res Lett. 2009; 4(12): 1452–1457.

Published online 2009 September 18. doi: 10.1007/s11671-009-9419-2

PMCID: PMC2893785

PX Yan: nc.ude.uzl@nayxp

Received 2009 June 18; Accepted 2009 August 12.

Copyright ©2009 to the authors

In this article, SnO_{2}nanowires (NWs) have been prepared and their microwave absorption properties have been investigated in detail. Complex permittivity and permeability of the SnO_{2}NWs/paraffin composites have been measured in a frequency range of 0.1–18 GHz, and the measured results are compared with that calculated from effective medium theory. The value of maximum reflection loss for the composites with 20 vol.% SnO_{2}NWs is approximately −32.5 dB at 14 GHz with a thickness of 5.0 mm.

In recent years, electromagnetic (EM) wave absorbing materials have aroused great interest because of more and more civil, commercial, and military applications in electromagnetic interference (EMI) shielding and radar cross section (RCS) reduction in the gigahertz (GHz) band range [1,2]. Traditionally, EM wave absorbing materials, which are composed of magnetic metals or alloys particles, are restricted in application because of high specific gravity and formulation difficulty. It is hence desirable to have microwave absorbing materials that are lightweight, structurally sound, and flexible and show good microwave-absorbing ability in a wide frequency range. In terms of these criteria, one-dimensional nanostructures, which have a tremendous surface area and more dangling bond atoms on surface, appear to be good candidates [3]. Recently, carbon nanotubes (CNTs) [4-6], magnetic-particle-doped CNTs [7], magnetic nanowires (NWs) [8], nanostructured ZnO [9,10], and Mn_{3}O_{4}[11] were intensively studied and found to be promising microwave absorbing materials. Many groups found ZnO nanomaterials with different morphologies show excellent microwave absorption behavior, and partly attributed to its semiconductor character [9,10,12]. Microwave absorption property of ZnO has been investigated thoroughly in previous reports. In this work, microwave absorption behavior of another important semiconductor SnO_{2} was investigated in detail.

SnO_{2} has been paid attention in a variety of applications in chemical, optical, electronic, and mechanical fields, due to its unique high conductivity, chemical stability, photoluminescence, and gas sensitivity [13-16]. However, the research on its dielectric property and microwave absorption has not been reported. Here, both the complex permittivity (ε_{r} = ε′ − *j*ε″) and permeability (μ_{r} = μ′ − *j*μ″) of the SnO_{2} NWs/paraffin composites with different loading proportion were studied, and the measured results are compared with calculation results from effective medium theory (EMT). The effective permittivity of composite has linear increase with increment of SnO_{2} NWs proportion. Their microwave reflection loss curves were simulated according to transmission line theory. The excellent absorbing properties of the NW–paraffin were revealed, and the relationship between absorption property and the proportion between SnO_{2} NWs and paraffin were also investigated.

SnO_{2}NWs were prepared by a normal chemical vapor deposition (CVD) method. Briefly, a small amount of Sn powder (purity: ≥99%, about 3 g) was placed in an alumina crucible. A porous aluminum oxide (AAO) template coated with Au film of about 10 nm was used as substrate, which was positioned about 5 cm downstream from the precursor. Then, the crucible was put into a quartz tube that was located at the center of an electronic resistance furnace. One end of the quartz tube was connected with a mass-flow controller, which introduces a constant mixed carrier gas flow of Ar and O_{2}at a flow rate of 100 and 10 sccm, respectively; the other end of the quartz tube was evacuated by a pump. The furnace was heated to 1,000 °C and kept for 1 h. After the furnace was cooled naturally down to room temperature, white wool-like products in high yield were found on the substrate.

The powder samples were characterized by high resolution transmission electron microscopy (TEM) and selected-area electron diffraction (SAED) on a JEM-2010 transmission electron microscope operated at 100 kV. Field emission scanning electron microscopy (FESEM) observation was performed on a Hitachi S-4800 field emission scanning electron microscope. The products were mixed with paraffin wax with different volume fraction and pressed into toroidal-shaped samples (_{out} = 7 mm, _{in} = 3*.*04 mm) for microwave absorption tests. The real part and imaginary part of the complex permittivity and permeability of the samples were measured using the transmission/reflection coaxial method by an Agilent E8363B vector network analyzer working at 0.1–18 GHz.

Figure Figure1shows1shows the SEM and TEM images of the as-synthesized SnO_{2}NWs. The diameters of the SnO_{2}NWs are about 100 nm, and the lengths are up to micron scale. From TEM image (Fig. (Fig.1c)1c) and HRTEM image (Fig. (Fig.1d),1d), as-synthesized SnO_{2}NWs are well crystallized and have smooth surfaces.

Figure Figure2is2is the typical SEM image of the SnO_{2}NWs/paraffin composite with 50 vol.% loading. From Fig. Fig.2a,2a, it is clear that the inclination angle of these NWs (indicated with arrows) in the composites is different, leading to the randomly oriented NWs in the composites, and the volume proportion of NWs close to the surface is much lower than 50%, which is lower than that inside the composites (indicated with ellipse in a gap). As paraffin is EM wave transparent, EM waves can easily penetrate into the microwave absorbing materials with this structure.

We independently measured the relative complex permittivity and permeability of the SnO_{2}NWs/paraffin composites in a frequency range of 2–18 GHz (Fig. (Fig.3a–c)3a–c) using the*T*/*R*coaxial line method as described in the experimental section. The complex permittivity of composite versus frequency is shown in Fig. Fig.3a.3a. One can see a decrease of ε′ and an increase of ε″ with frequency rise. It reveals that the real part ε′ exhibits an abrupt decrease from 23 to 18 at the 0–4-GHz range, an approximate constant over 4–12 GHz and a broad peak at 12–18 GHz. Meanwhile, the imaginary part increases from 0.1 to 0.5 in the whole frequency range. As shown in Fig. Fig.3b3b of complex permeability, a decrease of μ′ from 1.2 to 1 and an imaginary part close to 0 can be related to the absence of ferromagnetic components in the sample. The tangent of dielectric and magnetic loss can be expressed as tan δ_{E} = ε″/ε′ and tan*δ*_{M} = μ″/μ′, respectively. From Fig. 3a-b, it can be seen that tan δ_{E}increases from 0.1 to 0.5 in the whole frequency range, while tan δ_{M}is below 0.1. It suggests that microwave absorption enhancement of composite results mainly from dielectric loss rather than magnetic loss.

According to the transmission line theory [17], the normalized input impedance *Z*_{in} of a microwave absorber is given by

(1)

where μ_{r} and ε_{r} are the relative permeability and permittivity of the composite medium, *c* the velocity of EM waves in free space, *f* the frequency of the microwave, and *d* the thickness of the absorber. The reflection loss is related to *Z*_{in} as

(2)

where is the characteristic impedance of free space.

Figure Figure3c3c shows the microwave reflection loss of composite with 50 vol.% loading at different composite thicknesses. With matching thickness*t*_{m} = 7 mm, the maximum reflection loss*R*_{max}is ca. −16 dB at 7 GHz. At*t* = 2 mm, the bandwidth corresponding to reflection loss below −10 dB (i.e., over 90% microwave absorption) is higher than 1.5 GHz.

It can be seen that the sample of 50% proportion does not exhibit good ability of microwave absorption compared with the results of ZnO and CNTs [5-11], in order to find optimal loading proportion and to investigate the intrinsic reasons for the absorption. Figure Figure4a,4a, b show the real part ε′ and the imaginary part ε″ of the permittivity of the composite samples with different contents of SnO_{2} NWs. It can be seen that the values of both real part ε′ and imaginary part ε″ of the permittivity increase significantly with SnO_{2} NWs loading increasing, and the variation curve of every contents has the similar shape with that of 50 vol.%. Figure Figure4c–f4c–f shows the microwave reflection loss of composite with different loading proportion at different composite thicknesses. Composite of 10, 20, 30, and 40 vol.% loading proportion have their matching thickness *t*_{m} = 7, 5, 7, 7 mm and the approximate maximum reflection loss *R*_{max} = −27.5, −32.5, −25, −18 dB. It can be found that the microwave absorption property of the SnO_{2} NW/paraffin composites becomes better with the decrease of proportion of SnO_{2} NWs and get optimal proportion at 20% when the best EM parameter matching realizes. In particular, the composite sample of 40 vol.% exhibits enhanced microwave absorption with an absorber thickness of 2 mm, which is same as that of 50 vol.% shown in Fig. Fig.33c.

The dominant dipolar polarization and the associated relaxation phenomena of SnO_{2} constitute the loss mechanisms. Composite materials, in which semiconductor NWs are coated with a dielectric nanolayer, introduce additional interfaces and more polarization charges at the surface [18,19]. The interfacial polarization is an important polarization process and the associated relaxation will also give rise to a loss mechanism. It is reasonable to expect that the dielectric loss may be due to significant contributions of the interfacial polarization. It is well known that SnO_{2} NWs have excellent gas sensitivity and can form space charge layer of several nanometers on the surface. Molecular dipoles formed at the NWs surface interact with the microwave field, leading to some absorption losses through heating [18].

From Fig. Fig.4c–f,4c–f, it can be seen that composite of 10, 20, 30, 40 vol.% loading proportion have their approximate reflection loss *R*_{max} at 11.5, 10, 8.5, 8 GHz at thickness *t* = 7 mm. With the increase of proportion in the nanocomposites, the matching frequency tends to shift to the lower frequency region, and similar results have been gained on CNTs [1,2] and ZnO NWs [9]. Fan et al. pointed out that with an increase of CNT content in composite, the electric field of short-distance resonance multipoles leads to dominance of reflection property rather than absorption property. They reported that ε increase with increasing CNT concentration, resulting in a shift of reflectivity peak toward lower frequency [2]. The revelation is important because it suggests that the range of absorption frequency can be easily tuned by changing the SnO_{2} NWs content of composites. Thus, wideband absorption could be achieved by coupling SnO_{2} NWs/paraffin layers of different SnO_{2} NWs contents. So, it is of great significance to calculate real and imaginary part of complex permittivity at different loading proportion of SnO_{2} NWs.

Composites consisting of metallic or semiconductor particles embedded in a dielectric matrix have been widely used and studied for years [20-22], but their physical properties are still not fully understood or unveiled. It would be extremely useful to predict the properties of composites once the properties of constituent components are known and extract the properties of constituents from the measured composite properties. If the composites are isotropic and homogeneous, this work could be done with EMTs. Classical EMTs are usually based on an equivalent dipole representation of the composite. The effective macroscopic EM properties of the composites are modeled on the effective dipole moments per unit volume, which is determined by the intrinsic dipole moment contributions of each constituent and their relative volume concentration [23]. Among EMTs, the Bruggeman (BG) formula is the most commonly used. In this work, the complex permittivity ε of SnO_{2} NWs/paraffin composites at microwave frequencies has been studied in the framework of the BG formula.

(3)

From formula (3), one can calculate Φ*e*, Φ*m* as follows:

(4)

(5)

Φ is either of the real part and imaginary part of the complex permittivity ε and complex permeability μ. Φ*e*, Φ*i*, Φ*m* correspond to the parameter of the effective medium, the insulator, and the semiconductor particles, respectively. *p* is the volume fractions of SnO_{2} NWs in the components. The insulator is paraffin in our experiment, real part and imaginary part of the complex permittivity are 2 and 0.01, respectively, as shown in Fig. Fig.4a,4a, b

Using the BG equation, the effective permittivity of the SnO_{2}NWs/paraffin composite at 100 MHz was calculated over a wide particle volume fraction range of 10–50% and was compared to the measured values in Fig. Fig.5.5. Prior to the calculation, the permittivity of SnO_{2}NWs at 100 MHz was extracted from the measured effective permittivity of a mixture sample with SnO_{2}NWs of 40 vol.% using Eq. 4.

Comparison between the calculated and measured effective permittivity:**a**real part and**b**imaginary part of the composite at 100 MHz versus the volume fraction of SnO_{2}NWs

The real and the imaginary parts of the permittivity increase with the volume concentration. Our measured results show approximately a homogeneous increase across different proportion. BG formula predicts a distinct increase happening at around 30 vol.%, which results from the semiconductor–insulator transition at the percolation threshold [3], and a linear increase after percolation, which is the same as measured results but with a different slope. BG formula is often used in the case of spherical inclusions whose diameter *d* is much smaller than the incident wavelength λ. In our experiment, SnO_{2} NWs are around 100 nm in width and up to micron scale in length; the aspect ratio is so large that error may be brought and result in the difference in slope. As BG formula has difficulty in dealing with composite with percolation, we find that EMT can be only used in qualitative analyses, and leads to large error in quantitative analyses.

In conclusion, SnO_{2}NWs have been prepared by a CVD method and their microwave absorption properties have been investigated in detail. Complex permittivity and permeability of the SnO_{2}nanostructures and paraffin composites have been measured in a frequency range of 0.1–18 GHz, the value of both real part ε′ and imaginary part ε″ of the permittivity increase significantly with increasing SnO_{2}NWs loading, and the variation curve of every content has the similar shape. The value of maximum reflection loss for the composites with 20 vol.% SnO_{2}NWs is −32.5 dB at 14 GHz with a thickness of 5.0 mm. The measured results are compared with results calculated with EMT. We find that BG equation can be only used in qualitative analyses, and leads to large error in quantitative analyses.

- Liu ZF, Bai G, Huang Y, Li FF, Ma YF, Guo TY, He XB, Lin X, Gao HJ, Chen YS. J. Phys. Chem. C. 2007. p. 13696. COI number [1:CAS:528:DC%2BD2sXpsFyht7Y%3D] [Cross Ref]
- Tang NJ, Zhong W, Au C, Yang Y, Han MG, Lin KJ, Du YW. J. Phys. Chem. C. 2008. p. 19316. COI number [1:CAS:528:DC%2BD1cXhtlKqtL%2FJ] [Cross Ref]
- Qiu JX, Shen HG, Gu MY. Powder Technol. 2005. p. 116. COI number [1:CAS:528:DC%2BD2MXlvFejs7g%3D] [Cross Ref]
- Wadhawan A, Garrett D, Perez JM. Appl. 2003. p. 2683. COI number [1:CAS:528:DC%2BD3sXns1Cgs74%3D]; Bibcode number [2003ApPhL..83.2683W] [Cross Ref]
- Paton KR, Windle AH. Carbon. 2008. p. 46.
- Makeiff DA, Huber T. Synth. 2006. p. 156.
- Fan ZJ, Luo GH, Zhang ZF, Zhou L, Wei F. Mater. Sci. Eng. B. 2006. p. 85. COI number [1:CAS:528:DC%2BD28XotV2hsbY%3D] [Cross Ref]
- Encinas A, Vila L, Darques M, George JM, Piraux L. Nanotechnology. 2007. p. 065705. Bibcode number [2007Nanot..18f5705E] [Cross Ref]
- Zhuo RF, Feng HT, Chen JT, Yan D, Feng JJ, Li HJ, Geng BS, Cheng S, Xu XY, Yan PX. J. Phys. Chem. C. 2008. p. 11767. COI number [1:CAS:528:DC%2BD1cXosF2gs7o%3D] [Cross Ref]
- Zhuo RF, Feng HT, Liang Q, Liu JZ, Chen JT, Yan D, Feng JJ, Li HJ, Cheng S, Geng BS, Xu XY, Wang J, Wu ZG, Yan PX, Yue GH. J. 2008. p. 185405. Bibcode number [2008JPhD...41r5405Z] [Cross Ref]
- Yan D, Cheng S, Zhuo RF, Chen JT, Feng JJ, Feng HT, Li HJ, Wu ZG, Wang J, Yan PX. Nanotechnology. 2009. p. 105706. COI number [1:STN:280:DC%2BD1Mzitl2isw%3D%3D]; Bibcode number [2009Nanot..20j5706Y] [PubMed] [Cross Ref]
- Liu XG, Geng DY, Meng H, Shang PJ, Zhang ZD. Appl. 2008. p. 173117. Bibcode number [2008ApPhL..92q3117L] [Cross Ref]
- Wang Y, Lee JY, Deivaraj TC. J. Phys. Chem. B. 2004. p. 13589. COI number [1:CAS:528:DC%2BD2cXmslSnsb4%3D] [Cross Ref]
- Gao T, Wang T. Mater. 2008. p. 836. COI number [1:CAS:528:DC%2BD1cXislGkt7c%3D] [Cross Ref]
- Chen JT, Wang J, Zhang F, Yan D, Zhang GA, Zhuo RF, Yan PX. J. 2008. p. 105306. Bibcode number [2008JPhD...41j5306C] [Cross Ref]
- Mu J, Liu LY, Kang SZ. Nanoscale Res. 2007. p. 100. COI number [1:CAS:528:DC%2BD2sXktVart7o%3D]; Bibcode number [2007NRL.....2..100M] [Cross Ref]
- Natio Y, Suetake K. IEEE Trans. 1971. p. 65. [Cross Ref]
- Chen YJ, Cao MS, Wang TH, Wan Q. Appl. 2004. p. 26. Bibcode number [2004ApPhL..84...28C]
- Cao MS, Shi XL, Fang XY, Jin HB, Hou ZL, Zhou W. Appl. 2007. p. 203110. Bibcode number [2007ApPhL..91t3110C] [Cross Ref]
- Meng B, Klein BDB, Booske JH, Cooper RF. Phys. Rev. B. 1996. p. 12777. COI number [1:CAS:528:DyaK28XjtFCgt7s%3D]; Bibcode number [1996PhRvB..5312777M] [PubMed] [Cross Ref]
- Spivak B, Zhou F, Monod MTB. Phys. Rev. B. 1995. p. 13226. COI number [1:CAS:528:DyaK2MXlvVGru70%3D]; Bibcode number [1995PhRvB..5113226S] [PubMed] [Cross Ref]
- Studenikin SA, Potemski M, Sachrajda A, Hilke M, Pfeiffer LN, West KW. Phys. Rev. B. 2005. p. 245313. Bibcode number [2005PhRvB..71x5313S] [Cross Ref]
- Chen P, Wu RX, Zhao TE, Yang F, Xiao JQ. J. 2005. p. 2302. COI number [1:CAS:528:DC%2BD2MXmvFCntLk%3D]; Bibcode number [2005JPhD...38.2302C] [Cross Ref]

Articles from Nanoscale Research Letters are provided here courtesy of **Springer**

PubMed Central Canada is a service of the Canadian Institutes of Health Research (CIHR) working in partnership with the National Research Council's national science library in cooperation with the National Center for Biotechnology Information at the U.S. National Library of Medicine(NCBI/NLM). It includes content provided to the PubMed Central International archive by participating publishers. |